```Lecture Slides
Chapter 6
Fatigue Failure Resulting
Chapter Outline
Shigley’s Mechanical Engineering Design


Thus far we’ve studied STATIC FAILURE of machine elements.
The second major class of component failure is due to DYNAMIC LOADING
 Repeated stresses
 Alternating stresses
 Fluctuating stresses



The ultimate strength of a material (Su) is the maximum stress a material
can sustain before failure assuming the load is applied only once and
held.
A material can also FAIL by being loaded repeatedly to a stress level that
is LESS than (Su)
 Fatigue failure
Shigley’s Mechanical Engineering Design

Crack Initiation
 Fatigue always begins at a crack
 Crack may start at a microscopic
inclusion (&lt;.010 in.)
 Crack may start at a &quot;notch&quot;, or other
stress concentration

Crack Propagation
 Sharp crack creates a stress
concentration
 Each tensile stress cycle causes the
crack to grow
(~10-8 to 10-4 in/cycle)

Fracture
 Sudden, catastrophic failure with no
warning.
Stages of Fatigue Failure
Stage I – Initiation of microcrack due to cyclic plastic
deformation
 Stage II – Progresses to
macro-crack that repeatedly
opens and closes, creating
bands called beach marks
 Stage III – Crack has
propagated far enough that
remaining material is
and fails by simple ultimate
failure

Fig. 6–1
Shigley’s Mechanical Engineering Design
Schematics of Fatigue Fracture Surfaces
Fig. 6–2
Shigley’s Mechanical Engineering Design
Schematics of Fatigue Fracture Surfaces
Schematics of fatigue
fracture surfaces
produced in smooth
and notched
components with
round and rectangular
cross sections under
conditions and
nominal stress levels.
Fig. 6–2
Shigley’s Mechanical Engineering Design
Schematics of Fatigue Fracture Surfaces
Fig. 6–2
Shigley’s Mechanical Engineering Design
Fatigue Fracture Examples



AISI 4320 drive
shaft
B– crack initiation at
stress concentration
in keyway
C– Final brittle
failure
Fig. 6–3
Shigley’s Mechanical Engineering Design
Fatigue Fracture Examples


Fatigue failure
initiating at
mismatched grease
holes
Sharp corners (at
arrows) provided
stress concentrations
Fig. 6–4
Shigley’s Mechanical Engineering Design
Fatigue Fracture Examples



Fatigue failure of
forged connecting rod
Crack initiated at flash
line of the forging at the
left edge of picture
Beach marks show
crack propagation
halfway around the hole
before ultimate fracture
Fig. 6–5
Shigley’s Mechanical Engineering Design
Fatigue Fracture Examples




Fatigue failure of a
200-mm diameter
piston rod of an alloy
steel steam hammer
Crack initiated at a
forging flake internal to
the part
Internal crack grew
outward symmetrically
Fig. 6–6
Shigley’s Mechanical Engineering Design
Fatigue Fracture Examples


Double-flange trailer wheel
Cracks initiated at stamp marks
Fig. 6–7
Shigley’s Mechanical Engineering Design
Fatigue Fracture Examples

Aluminum allow landing-gear torque-arm assembly redesign to
eliminate fatigue fracture at lubrication hole
Fig. 6–8
Shigley’s Mechanical Engineering Design
Fatigue-Life Methods

Three major fatigue life models

Methods predict life in number of cycles to failure, N, for a specific level of loading

Stress-life method (S-N Curves)
◦ Least accurate, particularly for low cycle applications
◦ Most traditional, easiest to implement

Strain-life method (ε-N Curve)
◦ Detailed analysis of plastic deformation at localized regions
◦ Several idealizations are compounded, leading to uncertainties in results

Linear-elastic fracture mechanics method
◦ Assumes crack exists
◦ Predicts crack growth with respect to stress intensity
The above methods predict the life in number of cycles to failure, N, for a specific level
1.
Low cycle Fatigue:
2.
High cycle fatigue
Shigley’s Mechanical Engineering Design
Stress-Life Method





Test specimens are subjected to repeated stress while counting cycles
to failure
Most common test machine is R. R. Moore high-speed rotating-beam
machine
Subjects specimen to pure bending with no transverse shear
As specimen rotates, stress fluctuates between equal magnitudes of
tension and compression, known as completely reversed stress cycling
Specimen is carefully machined and polished
Fig. 6–9
Shigley’s Mechanical Engineering Design
S-N Diagram



Number of cycles to failure at varying stress levels is plotted on loglog scale
For steels, a knee occurs near 106 cycles
Strength corresponding to the knee is called endurance limit Se
Fig. 6–10
Shigley’s Mechanical Engineering Design
S-N Diagram for Steel



Stress levels below Se predict infinite life
Between 103 and 106 cycles, finite life is predicted
Below 103 cycles is known as low cycle, and is often considered
quasi-static. Yielding usually occurs before fatigue in this zone.
Fig. 6–10
Shigley’s Mechanical Engineering Design
S-N Diagram for Nonferrous Metals
Nonferrous metals often do not have an endurance limit.
 Fatigue strength Sf is reported at a specific number of cycles
 Figure 6–11 shows typical S-N diagram for aluminums

Fig. 6–11
Shigley’s Mechanical Engineering Design
Strain-Life Method
Method uses detailed analysis of plastic deformation at localized
regions
 Compounding of several idealizations leads to significant
uncertainties in numerical results
 Useful for explaining nature of fatigue

Shigley’s Mechanical Engineering Design
Strain-Life Method
Fatigue failure almost
always begins at a local
discontinuity
 When stress at
discontinuity exceeds
elastic limit, plastic
strain occurs
 Cyclic plastic strain can
change elastic limit,
 Fig. 6–12 shows true
stress-true strain
hysteresis loops of the
first five stress reversals

Fig. 6–12
Shigley’s Mechanical Engineering Design
Relation of Fatigue Life to Strain
Figure 6–13 plots relationship of fatigue life to true-strain
amplitude
 Fatigue ductility coefficient e'F is true strain corresponding to
fracture in one reversal (point A in Fig. 6–12)
 Fatigue strength coefficient s'F is true stress corresponding to
fracture in one reversal (point A in Fig. 6–12)

Fig. 6–13
Shigley’s Mechanical Engineering Design
Relation of Fatigue Life to Strain


Fatigue ductility exponent c is the slope of plastic-strain line, and is
the power to which the life 2N must be raised to be proportional to the
true plastic-strain amplitude. Note that 2N stress reversals corresponds
to N cycles.
Fatigue strength exponent b is the slope of the elastic-strain line, and
is the power to which the life 2N must be raised to be proportional to
the true-stress amplitude.
Fig. 6–13
Shigley’s Mechanical Engineering Design
Relation of Fatigue Life to Strain

Total strain is sum of elastic and plastic strain
Total strain amplitude is half the total strain range

The equation of the plastic-strain line in Fig. 6–13

The equation of the elastic strain line in Fig. 6–13

Applying Eq. (a), the total-strain amplitude is

Shigley’s Mechanical Engineering Design
Relation of Fatigue Life to Strain
Known as Manson-Coffin relationship between fatigue life and
total strain
 Some values of coefficients and exponents given in Table A–23
 Equation has limited use for design since values for total strain at

Shigley’s Mechanical Engineering Design
Linear-Elastic Fracture Mechanics Method
◦ Assumes Stage I fatigue (crack initiation) has occurred
◦ Predicts crack growth in Stage II with respect to stress
intensity
◦ Stage III ultimate fracture occurs when the stress intensity
factor KI reaches some critical level KIc
Shigley’s Mechanical Engineering Design
Stress Intensity Modification Factor
Stress intensity factor KI is a function of geometry, size, and
 For various load and geometric configurations, a stress intensity
modification factor b can be incorporated



Tables for b are available in the literature
Figures 5−25 to 5−30 present some common configurations
Shigley’s Mechanical Engineering Design
Crack Growth
Stress intensity factor

Stress intensity factor is given by

For a stress range Ds, the stress intensity range per cycle is

Testing specimens at various levels of Ds provide plots of crack
length vs. stress cycles
Stress intensity
modification factor
Fig. 6–14
Shigley’s Mechanical Engineering Design
Crack Growth



Log-log plot of rate
of crack growth,
da/dN, shows all
three stages of
growth
Stage II data are
linear on log-log
scale
Similar curves can
be generated by
changing the stress
ratio R = smin/ smax
Fig. 6–15
Shigley’s Mechanical Engineering Design
Crack Growth

Crack growth in Region II is approximated by the Paris equation

C and m are empirical material constants. Conservative
representative values are shown in Table 6–1.
Shigley’s Mechanical Engineering Design
Crack Growth

Substituting Eq. (6–4) into Eq. (6–5) and integrating,
ai is the initial crack length
 af is the final crack length corresponding to failure
 Nf is the estimated number of cycles to produce a failure after the
initial crack is formed

Shigley’s Mechanical Engineering Design
Crack Growth

If b is not constant, then the following numerical integration
algorithm can be used.
Shigley’s Mechanical Engineering Design
Example 6-1
Fig. 6–16
Shigley’s Mechanical Engineering Design
Example 6-1
Shigley’s Mechanical Engineering Design
Example 6-1
Fig. 5–27
Shigley’s Mechanical Engineering Design
Example 6-1
Shigley’s Mechanical Engineering Design
The Endurance Limit

The endurance limit for steels has been experimentally found to be
related to the ultimate strength
Shigley’s Mechanical Engineering Design
The Endurance Limit

Simplified estimate of endurance limit for steels for the rotatingbeam specimen, S'e
Shigley’s Mechanical Engineering Design
Fatigue Strength
For design, an approximation of the idealized S-N diagram is
desirable.
 To estimate the fatigue strength at 103 cycles, start with Eq. (6-2)


Define the specimen fatigue strength at a specific number of
cycles as

Combine with Eq. (6–2),
Shigley’s Mechanical Engineering Design
Fatigue Strength
At 103 cycles,
 f is the fraction of Sut represented by ( S f )103
 Solving for f,


The SAE approximation for steels with HB ≤ 500 may be used.

To find b, substitute the endurance strength and corresponding
cycles into Eq. (6–9) and solve for b
Shigley’s Mechanical Engineering Design
Fatigue Strength

Eqs. (6–11) and (6–12) can be substituted into Eqs. (6–9) and
(6–10) to obtain expressions for S'f and f
Shigley’s Mechanical Engineering Design
Fatigue Strength Fraction f
Plot Eq. (6–10) for the fatigue strength fraction f of Sut at 103
cycles
 Use f from plot for S'f = f Sut at 103 cycles on S-N diagram
 Assumes Se = S'e= 0.5Sut at 106 cycles

Fig. 6–18
Shigley’s Mechanical Engineering Design
Equations for S-N Diagram
Write equation for S-N
line from 103 to 106 cycles
 Two known points
 At N =103 cycles,
Sf = f Sut
 At N =106 cycles,
Sf = Se
 Equations for line:

Shigley’s Mechanical Engineering Design
Equations for S-N Diagram

If a completely reversed stress srev is given, setting Sf = srev in
Eq. (6–13) and solving for N gives,
Note that the typical S-N diagram is only applicable for
completely reversed stresses
 For other stress situations, a completely reversed stress with the
same life expectancy must be used on the S-N diagram

Shigley’s Mechanical Engineering Design
Low-cycle Fatigue
Low-cycle fatigue is defined for fatigue failures in the range
1 ≤ N ≤ 103
 On the idealized S-N diagram on a log-log scale, failure is
predicted by a straight line between two points (103, f Sut) and
(1, Sut)

Shigley’s Mechanical Engineering Design
Example 6-2
Shigley’s Mechanical Engineering Design
Example 6-2
Shigley’s Mechanical Engineering Design
Endurance Limit Modifying Factors
Endurance limit S'e is for carefully prepared and tested specimen
 If warranted, Se is obtained from testing of actual parts
 When testing of actual parts is not practical, a set of Marin
factors are used to adjust the endurance limit

Shigley’s Mechanical Engineering Design
Surface Factor ka
Stresses tend to be high at the surface
 Surface finish has an impact on initiation of cracks at localized
stress concentrations
 Surface factor is a function of ultimate strength. Higher strengths
are more sensitive to rough surfaces.

Shigley’s Mechanical Engineering Design
Example 6-4
Shigley’s Mechanical Engineering Design
Size Factor kb
Larger parts have greater surface area at high stress levels
 Likelihood of crack initiation is higher
 Size factor is obtained from experimental data with wide scatter
 For bending and torsion loads, the trend of the size factor data
is given by



Applies only for round, rotating diameter
For axial load, there is no size effect, so kb = 1
Shigley’s Mechanical Engineering Design
Size Factor kb
For parts that are not round and rotating, an
equivalent round rotating diameter is obtained.
 Equate the volume of material stressed at and above
95% of the maximum stress to the same volume in
the rotating-beam specimen.
 Lengths cancel, so equate the areas.
 For a rotating round section, the 95% stress area is
the area of a ring,


Equate 95% stress area for other conditions to Eq.
(6–22) and solve for d as the equivalent round
rotating diameter
Shigley’s Mechanical Engineering Design
Size Factor kb

For non-rotating round,

Equating to Eq. (6-22) and solving for equivalent diameter,

Similarly, for rectangular section h x b, A95s = 0.05 hb. Equating
to Eq. (6–22),

Other common cross sections are given in Table 6–3
Shigley’s Mechanical Engineering Design
Size Factor kb
Table 6–3
A95s for common
non-rotating
structural shapes
Shigley’s Mechanical Engineering Design
Example 6-4
Shigley’s Mechanical Engineering Design


Accounts for changes in endurance limit for different types of fatigue
method (Sec. 6–14) when more than one load type is present.
Shigley’s Mechanical Engineering Design
Temperature Factor kd
Endurance limit appears to maintain same relation to ultimate
strength for elevated temperatures as at room temperature
 This relation is summarized in Table 6–4

Shigley’s Mechanical Engineering Design
Temperature Factor kd
If ultimate strength is known for operating temperature, then just
use that strength. Let kd = 1 and proceed as usual.
 If ultimate strength is known only at room temperature, then use
Table 6–4 to estimate ultimate strength at operating temperature.
With that strength, let kd = 1 and proceed as usual.
 Alternatively, use ultimate strength at room temperature and
apply temperature factor from Table 6–4 to the endurance limit.


A fourth-order polynomial curve fit of the underlying data of
Table 6–4 can be used in place of the table, if desired.
Shigley’s Mechanical Engineering Design
Example 6-5
Shigley’s Mechanical Engineering Design
Example 6-5
Shigley’s Mechanical Engineering Design
Reliability Factor ke
From Fig. 6–17, S'e = 0.5 Sut is typical of the data and represents
50% reliability.
 Reliability factor adjusts to other reliabilities.
 Only adjusts Fig. 6–17 assumption. Does not imply overall
reliability.

Fig. 6–17
Shigley’s Mechanical Engineering Design
Reliability Factor ke

Simply obtain ke for desired reliability from Table 6–5.
Table 6–5
Shigley’s Mechanical Engineering Design
Miscellaneous-Effects Factor kf



Reminder to consider other possible factors.
◦ Residual stresses
◦ Directional characteristics from cold working
◦ Case hardening
◦ Corrosion
◦ Surface conditioning, e.g. electrolytic plating and metal
spraying
◦ Cyclic Frequency
◦ Frettage Corrosion
Limited data is available.
May require research or testing.
Shigley’s Mechanical Engineering Design
Stress Concentration and Notch Sensitivity
 Obtain Kt as usual (e.g. Appendix A–15)
 For fatigue, some materials are not fully sensitive to Kt so a
reduced value can be used.
 Define Kf as the fatigue stress-concentration factor.
 Define q as notch sensitivity, ranging from 0 (not sensitive) to 1
(fully sensitive).

For q = 0, Kf = 1
 For q = 1, Kf = Kt

Shigley’s Mechanical Engineering Design
Notch Sensitivity


Then get Kf from Eq. (6–32): Kf = 1 + q( Kt – 1)
Fig. 6–20
Shigley’s Mechanical Engineering Design
Notch Sensitivity



Then get Kfs from Eq. (6–32): Kfs = 1 + qs( Kts – 1)
Note that Fig. 6–21 is updated in 9th edition.
Fig. 6–21
Shigley’s Mechanical Engineering Design
Notch Sensitivity

Alternatively, can use curve fit equations for Figs. 6–20 and 6–21
to get notch sensitivity, or go directly to Kf .
Bending or axial:
Torsion:
Shigley’s Mechanical Engineering Design
Notch Sensitivity for Cast Irons
Cast irons are already full of discontinuities, which are included
in the strengths.
 Recommended to use q = 0.2 for cast irons.

Shigley’s Mechanical Engineering Design
Example 6-6
Shigley’s Mechanical Engineering Design
Shigley’s Mechanical Engineering Design
Application of Fatigue Stress Concentration Factor



Use Kf as a multiplier to increase the nominal stress.
Some designers (and previous editions of textbook) sometimes
applied 1/ Kf as a Marin factor to reduce Se .
For infinite life, either method is equivalent, since
1/ K f  Se

Se
nf 

K fs
s

For finite life, increasing stress is more conservative. Decreasing
Se applies more to high cycle than low cycle.
Shigley’s Mechanical Engineering Design
Example 6-8
Shigley’s Mechanical Engineering Design
Example 6-8
Shigley’s Mechanical Engineering Design
Example 6-8
Shigley’s Mechanical Engineering Design
Example 6-9
Fig. 6–22
Shigley’s Mechanical Engineering Design
Shigley’s Mechanical Engineering Design
&middot; Failure will probably occur at B rather
than C or at the point of maximum
bending moment.
&middot; Point B has:
- a smaller cross-section
- a higher bending moment
- a higher stress concentration
factor than C.
&middot; Location of the maximum bending
moment has a larger size and no stress
concentration.
Shigley’s Mechanical Engineering Design
Example 6-9
Bending
Room
Temp.
Shigley’s Mechanical Engineering Design
Example 6-9
Sut= 690Mpa = 100Kpsi,
notch radius = 3mm = 0.11 in
From Fig. 6.20, q = 0.84
Substituting into Eq. (6-32)
Kf = 1+q(Kt-1) = 1+0.84(1.65-1) = 1.55
Shigley’s Mechanical Engineering Design
Example 6-9
Shigley’s Mechanical Engineering Design
Characterizing Fluctuating Stresses



The S-N diagram is applicable for completely reversed stresses
Other fluctuating stresses exist
Shigley’s Mechanical Engineering Design
Fluctuating Stresses
General
Fluctuating
Fluctuating stress with
high frequency ripple
Repeated
Nonsinusoidal
fluctuating stress
Completely
Reversed
Nonsinusoidal
fluctuating stress
Fig. 6–23
Shigley’s Mechanical Engineering Design
Characterizing Fluctuating Stresses


Fluctuating stresses can often
be characterized simply by the
minimum and maximum
stresses, smin and smax
component of stress
(sometimes called mean
stress) and sa as amplitude of
alternating component of
stress
Shigley’s Mechanical Engineering Design
Characterizing Fluctuating Stresses

Other useful definitions
include stress ratio
and amplitude ratio
Shigley’s Mechanical Engineering Design
 The steady, or static, stress is not the same
as the midrange stress.
 The steady stress may have any value
between σmin and σmin .
 The steady stress exists because of a fixed
 A helical compression spring is always loaded into a space shorter than
the free length of the spring.
 The stress created by this initial compression is called the steady, or
static, component of the stress.
 Equations (6-36) use symbols σa and σm as the stress
components at the location of scrutiny.
 In the absence of a notch, σa and σm are equal to
the nominal stresses σao and σmo induced by loads Fa and Fm , respectively.
 With a notch they are σa
= Kf σao and σm = Kf σmo , respectively.
Where Kf is fatigue stress concentration factor
 When the steady stress component is high enough to induce localized notch
yielding, the designer has problem.
 The first-cycle local yielding produces plastic strain and strainstrengthening.
 This is occurring at the location where fatigue crack nucleation and growth
are most likely.
Application of Kf for Fluctuating Stresses
 For
fluctuating loads at points with stress
concentration, the best approach is to design to
avoid all localized plastic strain.
 In
this case, Kf should be applied to both
alternating and midrange stress components.
 When
localized strain does occur, some methods
(nominal mean stress method and residual stress
method) recommend only applying Kf to the
alternating stress.
Saturday, November 11, 2017
Application of Kf for Fluctuating Stresses
 Dowling
method recommends applying Kf to the
alternating stress and Kfm to the mid-range stress,
where Kfm is
Saturday, November 11, 2017
Fatigue Failure for Fluctuating Stresses
Vary the sm and sa to learn about the fatigue resistance under
 Three common methods of plotting results follow.

Shigley’s Mechanical Engineering Design
Modified Goodman Diagram

It has midrange stress plotted along the
abscissa and all other components of
stress plotted on the ordinate, with
tension in the positive direction.

The endurance limit, fatigue strength, or
finite-life strength whichever applies, is
plotted on the ordinate above and below
the origin.

The midrange line is a 45o line from the
origin to the tensile strength of the part.
Fig. 6–24
Shigley’s Mechanical Engineering Design
Master Fatigue Diagram

Displays four stress components as well as two stress ratios
Fig. 6–26
Shigley’s Mechanical Engineering Design
Master Fatigue Diagram.
Master fatigue
diagram for AISI
4340 steel with
Sut = 158
Sy = 147 kpsi.
The stress
component at A
are
σmin = 20,
σ max = 120,
σ m = 70,
σ o = 50
all in kpsi
Plot of Alternating vs Midrange Stress
Probably most common and simple to use is the plot of sa vs sm
 Has gradually usurped the name of Goodman or Modified
Goodman diagram
 Modified Goodman line from Se to Sut is one simple representation
of the limiting boundary for infinite life

Shigley’s Mechanical Engineering Design
Plot of Alternating vs Midrange Stress
Experimental data on normalized plot of sa vs sm
 Demonstrates little effect of negative midrange stress

Fig. 6–25
Shigley’s Mechanical Engineering Design
Commonly Used Failure Criteria



Five commonly used failure criteria are shown
Gerber passes through the data
ASME-elliptic passes through data and incorporates rough
yielding check
Fig. 6–27
Shigley’s Mechanical Engineering Design
Commonly Used Failure Criteria
Modified Goodman is linear, so simple to use for design. It is
more conservative than Gerber.
 Soderberg provides a very conservative single check of both
fatigue and yielding.

Fig. 6–27
Shigley’s Mechanical Engineering Design
Commonly Used Failure Criteria


Langer line represents standard yield check.
It is equivalent to comparing maximum stress to yield strength.
Fig. 6–27
Shigley’s Mechanical Engineering Design
Equations for Commonly Used Failure Criteria
Intersecting a constant slope load line with each failure criteria
produces design equations
 n is the design factor or factor of safety for infinite fatigue life

Shigley’s Mechanical Engineering Design
Summarizing Tables for Failure Criteria
Tables 6–6 to 6–8 summarize the pertinent equations for
Modified Goodman, Gerber, ASME-elliptic, and Langer failure
criteria
 The first row gives fatigue criterion
 The second row gives yield criterion
 The third row gives the intersection of static and fatigue criteria
 The fourth row gives the equation for fatigue factor of safety
 The first column gives the intersecting equations
 The second column gives the coordinates of the intersection

Shigley’s Mechanical Engineering Design
Summarizing Table for Modified Goodman
Shigley’s Mechanical Engineering Design
Summarizing Table for Gerber
Shigley’s Mechanical Engineering Design
Summarizing Table for ASME-Elliptic
Shigley’s Mechanical Engineering Design
```